Microstructure and Mechanical Properties of Functionally Graded AlSi/MWCNT Composite Cylinders

Experimental fabrication of functionally graded Aluminum Silicon-carbon nanotubes (AlSi-MWCNT) reinforcement is significantly less, despite substantial theoretical interest. Many studies focused on axially layered functionally graded material because of ease of fabrication. Full advantage of AlSi-MWCNT functionally graded material only is taken when designed to the various shapes. In this research work, functionally graded cylinders were produced with 2wt% MWCNT at the outer surface to provide a complex and wear-resistant surface. The interior surface is soft with AlSi to provide elasticity. FGM1 sample indicates 112% and 11% increase in maximum tensile strength compared to AlSi and AlSi-MWCNT1wt%. FGM1 sample shows a 37% increase in elongation percentage compared to the AlSi-MWCNT1wt% composite. Test samples showing the typical nature of barrelling. FGM1 sample exhibits compressive strength of 237MPa, exceeding by 245% that of AlSi and by 3.5% that of AlSi-MWCNT1wt%. Three samples consider for each test. Hardness value ranges from 65HV at the core to 115HV at the outer surface. Hardness value Exceeds 56% in the outer layer compared to an inner region of FGM2.There is a proper bond between the layers, and the same demonstrate with properties of tensile, compressive, and hardness. OM with porosity, SEM with EDX evaluates to predict structural gradation in FGM cylinder.


Introduction
Functionally graded materials are superior advanced materials with tailoring properties for the customer end product. Properties alter by controlling the constituent base matrix and reinforcement materials, which conventional alloys and composites are not possible. Tailoring properties makes them suitable for overcoming a wide variety of demanding problems such as thermal gradation, thermal mismatch, toughness, wear, corrosion, and impact.
The mechanical component wherein interior is soft and outer layer is tough, and wear-resistant benefitted from functionally graded material is shafts, gears, cams, and bearings. MWCNT reinforced nanofiller functionally graded materials are the trending newest materials investigated 1,2,3 Determines the FGM beams subjected longitudinal modeling. FEA modeling of axially functionally graded CNT Reinforced Composite. 4 Material topology of functionally graded beams subjected to bilateral constraints. 5 Studied instability of thermomechanical loaded graphene reinforced functionally graded materials. Young's modulus of graphene-FGM composite determined using modified Halpin-Tsai model. 6 Functionally graded materials subjected to thermal shock resistance by considering (a) local tensile stress criterion, (b) thermal stress intensity factor criterion, and (c) hoop stress criterion. 7 Studies on Finite rotation multiple nodes (3 & 4) shell elements for functionally graded CNT-reinforced thin composite shells analysis. Reviewed FG-graphene reinforced composite structures, discuss mechanical properties, characteristics, and micro-mechanics model of FG-graphene composite. 6 carried out Fracture analysis of functionally graded material using extended element-free Galerkin method and digital image correlation technique; the experimental method helps fabricate a five-layered epoxy/glass FGM by hand layup process. 9 Carried out Fracture analysis of functionally graded material using extended element-free Galerkin method and digital image correlation technique; the experimental method helps fabricate a five-layered epoxy/glass FGM by hand layup process. 10 Fatigue behavior of FG-Ti-6Al-4V mesh structure fabricated by electron beam. 11 Reviewed mechanical properties of CNT reinforced functionally graded materials. 12 Carried out the analysis of wave propagation of CNT reinforced by FG-Composite cylindrical micro-shell using shear deformable shell theory and nonlocal strain gradient theory. 13 The modeling of functionally graded carbon nanotubes reinforced composite plates subjected to low-velocity impact with arbitrary geometry and general boundary conditions. 14 Studies on free vibration analysis and bending of FG-graphene vs CNT-reinforced composite plates. 15 Functionally graded-CNT cylindrical shell on dynamic buckling analyses of under axial power-law time-varying displacement load.1 6 Determines the temperature-dependent properties of functionally graded porous materials subjected to Thermoelastic analysis by a staggered finite volume method. 17 Functionally gradient brittle materials impact response characteristics and mesoevolution mechanism. 18 Three-dimensional flexural deformations of functionally graded material beams. Research carried out on functionally graded cylinders with radial gradation is significantly less; in this research work, the expensive CNT is provided on the surface to give hardness and strength. The interior remains soft to provide elasticity. The prepared material with geometry provides less cost, which offers powerful applications with lightweight, overall ductility, hard and wear-resistant surface desire: used in mechanical components of an automobile and aircraft.

Materials and Methods
Functionally graded cylinders fabricated by step by step procedure. The first step involves selecting materials such as atomized aluminum-silicon alloy powder with > 99% purity and Ni-coated MWCNTs (Hongwu Nanometer) and Aluminum silicon alloy powder constituents shown in Table.1 The average particle size of Aluminum silicon alloy powder is in the range of 50-70µm. Aluminum silicon alloy powder, ball-milled with Ni-coated MWCNTs having average diameters of 30-60nm and length of 1-2µm, the percentage of Nickel coated is <40% on MWCNTs in a Retsch PM-100 ball mill under argon atmosphere. Milling speed of 250rpm and 5:1 ball to powder weight ratio, milled for 5hours to avoid damage to Ni-coating and structure of the MWCNTs and acetone used to avoid cold welding of aluminum particles. Three composite concentrations prepare by dispersing 1wt%, 1.5wt%, and 2wt% MWCNT in the Aluminum silicon alloy powders. Two types of specimens fabricated one is Four-layer, and Twolayer sample prepare with an inner layer is milled Aluminum silicon alloy powder. The outer layer is Aluminum silicon alloy with MWCNTs variation (1, 1.5 & 2) weight percentage. Figure. 1 sample considered FG2 where Centre milled AlSi will act as ductility layer, whereas MWCNTs wt% varied very marginally to avoid a mismatch between layers. Three pieces fabricate to take the average of results. With a comparative test, AlSi-MWCNT nano-composites manufacture by same powder metallurgy route with varying MWCNT wt% by 1, 1.5 & 2. 3D mold spacer is a cylinder of length 75mm and outer diameter of 31mm. The internal pocket of a spacer divides with three pockets of diameter 23mm, 15mm, and 7mm separated with the minute thickness of 0.3mm. Each pocket provides three slots that aid in powder loading and rigidity to the mold. 3D mold spacer eliminates the use of lubricants, loading parts with mildew, and helps in avoiding contamination of the powders. The weighted percentages of each of the composition samples carefully pour using the small chimney. After filling, the mold is delicately removed from the cold compaction die to allow powders to fall in place and merge.
They are coarsening of particles due to cold welding in the ball milling process, clearly seen in Figure.3(a-d). SEM analysis indicates the uniform dispersion of MWCNTs in Aluminum silicon alloy particles, and in some parts, there is an agglomeration of bonded particles. AlSi-MWCNT particles showing irregular morphology and rough surfaces compared to AlSi. SEM images prove the effectiveness of ball milling parameters (Ball milling time, speed, BPR & PCA amounts) used in this research helps avoid MWCNT clusters. 20 The particle size, morphology, and composition of constituents influence the compaction and sintering of FGM cylinders, mainly helps in interfacial strength between the layers.

Optical Microscopy and Porosity
Optical microscopy of FGM sample with an inner layer is AlSi, and the outer layer is AlSi-MWCNT, there is no presence of crack between each layer as discussed by, 20 didn't occur in this research. The microstructure consists of uniformly dispersed eutectic silicon particles. Intermetallic phases in the inter-dendritic region in the matrix of aluminum solid solution. (~5-8%) Porosity observed in sample Fig.4(a). the layer of AlSi-1.5wt%MWCNT porosity reduces to 5% shown in Fig.4(b) and AlSi-2wt%MWCNT limited to 3% in Fig.4(c), it is a positive sign of good compaction and sintering. Uniform dispersion of multiwall carbon nanotubes (MWCNT) in AlSi matrix helps in reducing the porosity to an extent of weight percentage of 2wt%. [21][22][23] SEM analysis with EDX of FGM cylinders Sample No 1, AlSi + (1wt % Ni-MWCNT +AlSi) Fig. 4: (a-c) shows optical microscopy of FGM1 cylinder with respect to layers and Porosity in each layer. SEM images with EDX of AlSi with Ni coated MWCNT are seen in Figure.5 (a-c). SEM images indicating the uniform dispersion of MWCNTs in the Aluminum silicon alloy matrix with Ni content presence in EDX graph, and the same thing proved with weight percentage. Ni coating on MWCNTs helps improve the dispersion in the AlSi matrix. Proper uniform distribution helps enhance the properties of the FGM material, and the same is portray in tensile and compressive properties.

Mechanical Properties
The tensile test evaluates the mechanical behavior of FGM samples. Challenge occurs during machining of FGM sample to reduce cross-section. It will remove the outer part of the FGM layer, which consists of a higher concentration of MWCNT it would affect mechanical properties. FGM machined to the ASTM standard as shown in Figure.8 it is possible to reduce it to 14.5mm diameter, and grips, on the other hand, is 16mm as same been followed in. 19 FGM1 samples fracture to the middle of the gauge length. FGM1 sample fracture by the combined effect of ductile and brittle nature.

Conclusion
Research carried out on FGM cylinder is very little. Only axially layered FGMs were fabricated due to processing constraints. Theoretical studies indicate various shapes of FGM are fabricated such as conical shapes, panels, beams, discs, cylinders and plates. Present work demonstrates the FGM cylinders with radial CNT composition gradient.
Tensile test results predict FGM performs well compared to base AlSi, and AlSi-1wt%MWCNT provides a better combination between strength and ductility. Micro-Vickers hardness value indicates the outer surface is more hard compared to the core. The compressive properties of FGM cylinders provide more stability and sustainability compared to base AlSi and AlSi-1wt%MWCNT. Micro structural evaluation carries out with Optical microscopy with porosity, and SEM with EDX provides structural gradation of FGM layers.
The produced FGM cylinders provide the solution to a wide variety of challenges of drive shaft designs. It will provide toughness, strength, and lightweight.

Acknowledgement
Authors would like to thank Principal of constituent college for continuous support and encouragement.

Funding
There is no funding for this research work.

Conflict of Interest
There is no conflict of interest among authors.